THIN-SHELL CONCRETE FROM FABRIC MOLDS
La Ciucad Abierta (the Open City) Projecto Taller de Obras
by Mark West
technologies and instigations from
This article describes methods of forming prefabricated, fiber-reinforced, thin-shell concrete structures using molds made from hanging flat sheets of fabric. These fabric sheets are allowed to deflect into naturally occurring funicular geometries, producing molds for lightweight funicular compression vaults and double curvature wall panels.
These methods were developed to provide lightweight wall and floor structures for the Taller de Obras project, a new architectural atelier building at the Open City in Ritoque Chile, designed by architects Miguel Equem and David Jolly (seen above with a preliminary model of the building), in collaboration with the Centre for Architectural Structures and Technology (C.A.S.T.) Laboratory at the University of Manitobas Faculty of Architecture.
This document is presented in Three parts: 1: C.A.S.T.s proposals for the floor structure construction, including a brief overview of some of the architectural possibilities opened up by the ability to fabricate pre-cast funicular thin-shell vaults from fabric-formed molds; 2: a description of a method for fabricating double curvature thin-shell wall panels from hanging sheets of fabric; and 3: a gallery of photographs exploring some of the new architectural possibilities opened up by the research done for this project.
COMPRESSION VAULT FLOOR SLABUSING PRE-CAST THIN-SHELL PAN FORMWORK
PRODUCED FROM FABRIC-FORMED MOLDS
The Taller de Obras floor structure is a cast-in-place reinforced concrete slab supported by a 3 m by 3 m grid of supporting beams (plan below). This project proposes to reduce the amount of reinforcing steel this slab requires by using pre-cast thin-shell funicular vaults (approximately 3 m by 1 m), made from fiber-reinforced concrete to serve as stay-in-place formwork pans for a cast-in-place floor slab designed to span by compression between its integrally formed beams.
The production method for these pan formwork vaults is illustrated in the pages below
Floor structure viewed from below showing the pattern of individ-ual precast compres-sion vault formwork pans for a cast-in-place slab.
Reinforcing steel in integral valley beams
Prefabricated, fiber-re-inforced thin-shell com-pression vault formwork pans.
FIRST TEST OF FABRIC FORMED MOLD FOR PRODUCTION OF PRECAST THIN-SHELL FUNICULAR VAULTS
Lafarge Precast Factory, Winnipeg, Canada -- April 2004
1. A flat rectangular sheet of geotextile fabric is hung from a steel frame
2. A uniform thickness of Glass fiber Reinforced Concrete (GFRC) is applied to the hanging fabric.
3. The resulting funicular shell is inverted to make a mold for precast production.
4. A thin-shell GFRC vault is produced from the fabric-formed mold.
5. Plaster model of a precast funicular vault structure (supported here by fabric-formed prestressed plaster trusses). C.A.S.T. Laboratory 2007
SECOND TEST OF FABRIC FORMED MOLD FOR PRODUCTION OF PRECAST THIN-SHELL FUNICULAR VAULTS
Lafarge Precast Factory, Winnipeg, Canada -- April 2007
1. A simple open frame is constructed. We used 3/4 in (19 mm) plywood, built to the full-scale dimensions of the proposed Taller de Ob-ras formwork pans (1m x 3m opening).
2. A coated woven polyethylene fabric is stapled to 3/4 in. (19 mm) plywood strips and stretched over the opening to remove any wrin-kles that might form in the sheet.
3. The wood strips are screwed to the frame, thus fixing the fabric in place. A uniform thick-ness of fiber-reinforced concrete is placed over the fabric. In this case a sprayed shotcrete is used, but hand application of the concrete is also possible. The edges are reinforced with steel rebar.
4. The funicular shell thus formed is removed from the frame to be used as a plastic-coated mold for precast production of fiber-reinforced thin-shell funicular compression vaults. These vaults can be used directly as structure, or as stay-in-place formwork pans.
Woven high density polyethylene or polypro-pylene fabrics can be manufactured with a smooth waterproof coating on one side, and a fuzzy non-woven fabric welded to the other. If the concrete is applied to the non-woven side, the fabric will permanently adhere to it, providing a smooth, permanent, plastic-coated release surface for the mold.
Scaled physical models are excellent tools for developing and predicting practical techniques for full-scale fabric formwork construction. Based on 15 years of research experience, we have found that whatever we can build in scaled working models can be constructed at full-scale. The scaled compres-sion shell molds shown below illustrate a small sample of the vault forms that can be constructed using fl at sheets of fabric.
Closely following the methods developed for the Taller de Obras project, this model used a plastic-coated fabric sheet placed over a square opening (above left) to make a plastic-coated mold (above right). Three of the funicular compression vaults cast from this mold are shown below. These vaults require continuous support along all four edges because the original fabric sheet was itself continuously supported.
OTHER APPLICATIONS OF FABRIC-FORMED PRECAST COMPRESSION VAULTS
This mold (above left) was made by supporting a flat sheet of fabric from its four corners. The funicular shell cast from this mold (above right) resolves its compression forces to four point support at the cor-ners. Horizontal thrust forces can be contained by tension reinforcing integrated into the shell along its perimeter, connecting the four support points in a tension ring.
The mold (above left) was formed by a rectangular sheet of fabric that was pre-tensioned by pushing up-wards at two points (above right). The shells produced from this mold (at left) are cantilevered shells -- their lower surface is in compression and their upper sur-face is reinforced for tension.
It will be appreciated that a multitude of funicular vault forms can be produced by supporting a flat fabric sheet in different ways. The tension geometries as-sumed by the fabric under load will produce molds for funicular compression shells shaped to support the same (but reversed) loading patterns.
A mold for a vault designed to support uniform plus concentrated loads can be made by placing point loads on a flat fabric sheet (above left) prior to placing a uniform load of concrete. The result is the mold shown (above center) and the shell cast from this mold (above right). A shell such as this could support, for example, both its own dead-weight and that of a raised-floor structure placed upon it.
The flying vault shown below is formed by holding a flat fabric sheet from three points while pulling outwards on the fourth point ( below, top left). The mold formed by such a rig (below, middle left) pro-duces the vault shown below. This vault spans by resisting the precise inverse of the forces experi-enced by the loaded fabric membrane during the formation of the mold.
PRE-FABRICATED, THIN-SHELL WALL PANELS FORMED FROM HANGING SHEETS OF FABRIC
For the Taller de Obras Project, Open City, Ritoque Chile
The Taller de Obras building has twelve individual drawing cells placed around the perimeter of the floor slab. A full-scale mock-up of one of these cells, constructed of plywood at the Open City, is shown in the photos above. Reflected light is brought into the drawing space by a clerestory window and the curvature of the cell wall.
The drawings below show a proposal for fabric-formed thin-shell concrete panels to be used in these cells. These curved panels would be manufactured by the methods illustrated in the pages that follow.
THIN-SHELL PANELS CAST FROM SHEETS OF HANGING FABRICLafarge Precast Factory, Winnipeg, Canada -- April 2007
A hanging sheet of woven polyolefin geotextile fabric can be used as a mold to produce thin-shell wall panels. The panel shown above uses very little concrete. It is only 5 cm (2 in.) thick. The perimeter edges are 10 cm (4 in.) thick, reinforced with one 15 mm steel rebar on each of the four sides.
It gains its rigidity and strength from its deep folds and double cur-vatures. It is made by spraying a fiber-reinforced concrete against a hanging sheet of fabric.
This technology was developed at C.A.S.T. using small working models as illustrated in the three images below. A light nylon fabric was sprayed with wet plaster to form the models shown here. Our model fabric formwork rigs were scaled up for the full-scale tests. This kind of simple scaling up is possible because tension forces scale up linearly (as opposed, for example, to bending forces which increase geometrically, as the square of the span).
These tests used flat sheets of an un-coated woven polypropylene geotextile fabric as the formwork. Al-ternately, a fabric with a smooth plastic coating on one side and a fuzzy non-woven fabric heat welded to the other could be used, so that the hanging fabric would become permanently affixed to the con-crete. This would producing a plastic-covered mold to be used horizontally in the precast production of identical wall panels.
The surface of a small-scale plaster model (above left) is compared here with the surface of a full-scale shotcrete panel (above right).
The fabrication of one of these thin-shell fibre-reinforced panels is shown below (left) along with the finished panel (below right).
PLASTER WORKING MODELS - ILLUSTRATING PRECA